#------------------------------------------------------------------------------
#$Date: 2019-11-10 06:17:59 +0200 (Sun, 10 Nov 2019) $
#$Revision: 225696 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/51/55/4515539.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4515539
loop_
_publ_author_name
'Noh, Hyunho'
'Kung, Chung-Wei'
'Otake, Ken-ichi'
'Peters, Aaron W.'
'Li, Zhanyong'
'Liao, Yijun'
'Gong, Xinyi'
'Farha, Omar K.'
'Hupp, Joseph T.'
_publ_section_title
;
 Redox-Mediator-Assisted Electrocatalytic Hydrogen Evolution from Water by
 a Molybdenum Sulfide-Functionalized Metal--Organic Framework
;
_journal_issue                   10
_journal_name_full               'ACS Catalysis'
_journal_page_first              9848
_journal_paper_doi               10.1021/acscatal.8b02921
_journal_volume                  8
_journal_year                    2018
_chemical_formula_moiety         'C88 H44 O32 Zr6 (Mo O2)0.96'
_chemical_formula_sum            'C88 H44 Mo0.96 O32 S1.92 Zr6'
_chemical_formula_weight         2314.21
_space_group_crystal_system      hexagonal
_space_group_IT_number           191
_space_group_name_Hall           '-P 6 2'
_space_group_name_H-M_alt        'P 6/m m m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2017/1
_audit_update_record
;
2018-01-18 deposited with the CCDC.
2018-01-18 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   39.254(7)
_cell_length_b                   39.254(7)
_cell_length_c                   16.542(3)
_cell_measurement_reflns_used    340
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      14.41
_cell_measurement_theta_min      2.41
_cell_volume                     22074(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_publication_material  'Yadokari-XG (Wakita, Nemoto et al., 2009)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2500
_diffrn_reflns_av_unetI/netI     0.1530
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            16713
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        17.897
_diffrn_reflns_theta_max         17.897
_diffrn_reflns_theta_min         1.198
_diffrn_source                   'MoK\a I\mS microfocus source with MX Optics'
_exptl_absorpt_coefficient_mu    0.283
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.8762
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS-2014/5; Krause et al., 2015)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    0.522
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3417
_exptl_crystal_size_max          0.025
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.020
_refine_diff_density_max         0.590
_refine_diff_density_min         -0.462
_refine_diff_density_rms         0.095
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.081
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     179
_refine_ls_number_reflns         2899
_refine_ls_number_restraints     261
_refine_ls_restrained_S_all      1.054
_refine_ls_R_factor_all          0.1324
_refine_ls_R_factor_gt           0.0817
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1472P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2474
_refine_ls_wR_factor_ref         0.2833
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1565
_reflns_number_total             2899
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cs8b02921_si_003.cif
_cod_data_source_block           NU1000-MoSx-SIM
_cod_original_cell_volume        22074(9)
_cod_database_code               4515539
_shelx_shelxl_version_number     2017/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.6287
_shelx_estimated_absorpt_t_max   0.7450
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z'
'y, -x+y, z'
'x-y, -y, -z'
'-x, -x+y, -z'
'y, x, -z'
'-y, -x, -z'
'x, x-y, -z'
'-x+y, y, -z'
'-x, -y, -z'
'x, y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+y, -x, -z'
'-y, x-y, -z'
'-x+y, y, z'
'x, x-y, z'
'-y, -x, z'
'y, x, z'
'-x, -x+y, z'
'x-y, -y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.0941(5) 0.4921(5) 0.1336(11) 0.041(5) Uani 1 1 d . U . . .
C2 C 0.1237(5) 0.4905(5) 0.1855(10) 0.040(4) Uani 1 1 d . U . . .
C3 C 0.1132(5) 0.4600(5) 0.2427(9) 0.049(5) Uani 1 1 d . U . . .
H1 H 0.087220 0.440043 0.249358 0.059 Uiso 1 1 calc R U . . .
C4 C 0.1435(6) 0.4613(6) 0.2885(10) 0.065(6) Uani 1 1 d . U . . .
H2 H 0.136902 0.441957 0.327674 0.078 Uiso 1 1 calc R U . . .
C5 C 0.1824(5) 0.4890(6) 0.2798(10) 0.051(5) Uani 1 1 d . U . . .
C6 C 0.1918(5) 0.5180(5) 0.2224(10) 0.057(5) Uani 1 1 d . U . . .
H3 H 0.217922 0.537322 0.214894 0.068 Uiso 1 1 calc R U . . .
C7 C 0.1625(5) 0.5187(5) 0.1759(10) 0.056(5) Uani 1 1 d . U . . .
H4 H 0.169386 0.538439 0.137687 0.068 Uiso 1 1 calc R U . . .
C8 C 0.2445(4) 0.4890(7) 0.2893(15) 0.058(7) Uani 1 2 d S TU P . .
H5 H 0.244664 0.489330 0.233047 0.070 Uiso 1 2 calc R U P . .
C9 C 0.2147(5) 0.4888(6) 0.3254(10) 0.058(5) Uani 1 1 d . U . . .
C10 C 0.2135(5) 0.4890(6) 0.4090(11) 0.065(5) Uani 1 1 d . U . . .
C11 C 0.2440(4) 0.4880(7) 0.4532(13) 0.065(7) Uani 1 2 d S TU P . .
C12 C 0.1825(5) 0.4933(5) 0.4565(9) 0.083(6) Uani 1 1 d . U . . .
H6 H 0.163321 0.495922 0.428729 0.099 Uiso 1 1 calc R U . . .
O1 O 0.1047(3) 0.5184(3) 0.0820(6) 0.030(3) Uani 1 1 d . U . . .
O2 O 0.0577(3) 0.4654(3) 0.1500(6) 0.039(3) Uani 1 1 d . U . . .
O3 O 0.0348(4) 0.5174(2) 0.1097(9) 0.066(5) Uiso 1 2 d S . P A .
O4 O 0.0364(4) 0.4732(4) 0.000000 0.058(5) Uiso 1 2 d S . P A .
O5 O 0.000000 0.4006(4) 0.0737(12) 0.042(5) Uani 0.94 2 d S T P A 2
O6 O 0.000000 0.4680(5) 0.2376(8) 0.064(6) Uani 1 2 d S T P A .
Zr1 Zr 0.000000 0.45491(6) 0.10667(12) 0.0278(9) Uani 1 2 d DS T P A .
Zr2 Zr 0.07296(8) 0.53648(4) 0.000000 0.0207(10) Uani 1 4 d S T P . .
Mo3 Mo 0.000000 0.3876(15) 0.000000 0.148(18) Uani 0.12 4 d S TU P A 1
O7 O 0.000000 0.3991(6) 0.120(14) 0.01(10) Uiso 0.06 2 d DS . P A 1
Mo2 Mo -0.0245(16) 0.4877(8) 0.251(3) 0.156(18) Uani 0.08 2 d DS TU P . .
S3 S 0.000000 0.500000 0.382(7) 0.22(5) Uiso 0.16 4 d DS . P A .
S1 S 0.000000 0.342(3) 0.000000 0.19(3) Uiso 0.2 4 d DS . P A 2
Mo1 Mo -0.0355(15) 0.3843(16) 0.000000 0.20(2) Uani 0.1 2 d DS TU P A 2
S2 S -0.106(3) 0.316(3) 0.000000 0.19(3) Uiso 0.1 2 d DS . P A 2
S4 S -0.087(4) 0.456(2) 0.332(11) 0.22(5) Uiso 0.08 2 d DS . P A .
S5 S -0.034(5) 0.331(6) 0.000000 0.34(9) Uiso 0.12 2 d S . P A 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zr Zr -2.9673 0.5597 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 C1 O2 125.8(16) . .
O1 C1 C2 119.7(16) . .
O2 C1 C2 114.4(17) . .
C7 C2 C3 119.8(16) . .
C7 C2 C1 118.6(17) . .
C3 C2 C1 121.6(16) . .
C4 C3 C2 116.8(16) . .
C5 C4 C3 124.4(17) . .
C4 C5 C6 117.4(17) . .
C4 C5 C9 124.1(18) . .
C6 C5 C9 118.5(17) . .
C5 C6 C7 120.7(17) . .
C2 C7 C6 120.9(17) . .
C9 C8 C9 126(2) . 19
C8 C9 C10 119.1(18) . .
C8 C9 C5 122.2(16) . .
C10 C9 C5 118.7(15) . .
C9 C10 C11 119.0(16) . .
C9 C10 C12 122.9(15) . .
C11 C10 C12 117.9(16) . .
C10 C11 C10 118(2) . 19
C10 C11 C11 121.0(11) . 14_556
C10 C11 C11 121.0(11) 19 14_556
C12 C12 C10 120.9(9) 14_556 .
C1 O1 Zr2 133.5(11) . .
C1 O2 Zr1 133.6(10) . .
Zr1 O3 Zr1 112.4(7) 2_565 .
Zr1 O3 Zr2 107.7(5) 2_565 .
Zr1 O3 Zr2 107.7(5) . .
Zr1 O3 Mo2 86.6(9) 2_565 2_565
Zr1 O3 Mo2 86.6(9) . 2_565
Zr2 O3 Mo2 153.0(15) . 2_565
Zr1 O4 Zr1 110.0(7) 14 .
Zr1 O4 Zr2 109.4(5) 14 .
Zr1 O4 Zr2 109.4(5) . .
Zr1 O4 Mo1 89.4(9) 14 8
Zr1 O4 Mo1 89.4(9) . 8
Zr2 O4 Mo1 145.6(16) . 8
Mo1 O5 Mo1 89(3) 8 .
Mo1 O5 Zr1 98.3(19) 8 .
Mo1 O5 Zr1 98.3(19) . .
Mo2 O6 Mo2 66(4) 2_565 .
Mo2 O6 Zr1 109(2) 2_565 .
Mo2 O6 Zr1 109(2) . .
O3 Zr1 O3 67.5(7) 2_565 .
O3 Zr1 O4 72.4(5) 2_565 8
O3 Zr1 O4 109.6(5) . 8
O3 Zr1 O4 109.6(6) 2_565 .
O3 Zr1 O4 72.4(5) . .
O4 Zr1 O4 70.0(7) 8 .
O3 Zr1 O5 144.2(4) 2_565 .
O3 Zr1 O5 144.2(4) . .
O4 Zr1 O5 78.4(6) 8 .
O4 Zr1 O5 78.4(6) . .
O3 Zr1 O7 145.5(12) 2_565 .
O3 Zr1 O7 145.5(12) . .
O4 Zr1 O7 95(5) 8 .
O4 Zr1 O7 95(5) . .
O3 Zr1 O2 76.7(4) 2_565 23
O3 Zr1 O2 139.2(5) . 23
O4 Zr1 O2 76.0(4) 8 23
O4 Zr1 O2 140.9(4) . 23
O7 Zr1 O2 69.1(19) . 23
O3 Zr1 O2 139.2(5) 2_565 .
O3 Zr1 O2 76.7(4) . .
O4 Zr1 O2 140.9(4) 8 .
O4 Zr1 O2 76.0(4) . .
O5 Zr1 O2 76.4(3) . .
O7 Zr1 O2 69.1(19) . .
O2 Zr1 O2 125.2(5) 23 .
O3 Zr1 O6 77.6(6) 2_565 .
O3 Zr1 O6 77.6(6) . .
O4 Zr1 O6 142.8(4) 8 .
O4 Zr1 O6 142.8(4) . .
O5 Zr1 O6 117.7(7) . .
O7 Zr1 O6 98(6) . .
O2 Zr1 O6 76.1(3) 23 .
O2 Zr1 O6 76.1(3) . .
O3 Zr1 Mo1 144.9(8) 2_565 8
O3 Zr1 Mo1 111.5(10) . 8
O4 Zr1 Mo1 75.5(8) 8 8
O4 Zr1 Mo1 44.3(9) . 8
O7 Zr1 Mo1 51(5) . 8
O2 Zr1 Mo1 109.0(10) 23 8
O2 Zr1 Mo1 66.8(8) . 8
O6 Zr1 Mo1 137.5(7) . 8
O3 Zr1 Mo1 111.5(10) 2_565 .
O3 Zr1 Mo1 144.9(8) . .
O4 Zr1 Mo1 44.3(9) 8 .
O4 Zr1 Mo1 75.5(8) . .
O5 Zr1 Mo1 34.8(9) . .
O2 Zr1 Mo1 66.8(8) 23 .
O2 Zr1 Mo1 109.0(10) . .
O6 Zr1 Mo1 137.5(8) . .
Mo1 Zr1 Mo1 47.8(18) 8 .
O3 Zr1 Mo2 69.9(8) 2_565 2_565
O3 Zr1 Mo2 49.9(9) . 2_565
O4 Zr1 Mo2 141.9(8) 8 2_565
O4 Zr1 Mo2 118.5(10) . 2_565
O7 Zr1 Mo2 119(6) . 2_565
O2 Zr1 Mo2 100.1(10) 23 2_565
O2 Zr1 Mo2 72.3(9) . 2_565
O6 Zr1 Mo2 27.7(9) . 2_565
O4 Zr2 O4 109.6(8) . 20_565
O4 Zr2 O1 77.6(4) . .
O4 Zr2 O1 141.5(2) 20_565 .
O4 Zr2 O1 77.6(4) . 14
O4 Zr2 O1 141.5(2) 20_565 14
O1 Zr2 O1 76.6(5) . 14
O4 Zr2 O1 141.5(2) . 20_565
O4 Zr2 O1 77.6(4) 20_565 20_565
O1 Zr2 O1 75.2(5) . 20_565
O1 Zr2 O1 120.8(5) 14 20_565
O4 Zr2 O1 141.5(2) . 11_565
O4 Zr2 O1 77.6(4) 20_565 11_565
O1 Zr2 O1 120.8(5) . 11_565
O1 Zr2 O1 75.2(5) 14 11_565
O1 Zr2 O1 76.6(5) 20_565 11_565
O4 Zr2 O3 70.4(3) . .
O4 Zr2 O3 70.4(3) 20_565 .
O1 Zr2 O3 77.4(4) . .
O1 Zr2 O3 142.3(3) 14 .
O1 Zr2 O3 77.4(4) 20_565 .
O1 Zr2 O3 142.3(3) 11_565 .
O4 Zr2 O3 70.4(3) . 14
O4 Zr2 O3 70.4(3) 20_565 14
O1 Zr2 O3 142.3(3) . 14
O1 Zr2 O3 77.4(4) 14 14
O1 Zr2 O3 142.3(3) 20_565 14
O1 Zr2 O3 77.4(4) 11_565 14
O3 Zr2 O3 108.9(8) . 14
O4 Zr2 Zr1 35.2(2) . 14
O4 Zr2 Zr1 90.3(3) 20_565 14
O1 Zr2 Zr1 110.6(3) . 14
O1 Zr2 Zr1 74.4(3) 14 14
O1 Zr2 Zr1 164.8(3) 20_565 14
O1 Zr2 Zr1 110.1(2) 11_565 14
O3 Zr2 Zr1 89.9(3) . 14
O3 Zr2 Zr1 35.2(2) 14 14
O4 Zr2 Zr1 90.3(3) . 13_565
O4 Zr2 Zr1 35.2(2) 20_565 13_565
O1 Zr2 Zr1 164.8(3) . 13_565
O1 Zr2 Zr1 110.1(2) 14 13_565
O1 Zr2 Zr1 110.6(3) 20_565 13_565
O1 Zr2 Zr1 74.4(3) 11_565 13_565
O3 Zr2 Zr1 89.9(3) . 13_565
O3 Zr2 Zr1 35.2(2) 14 13_565
Zr1 Zr2 Zr1 60.36(8) 14 13_565
O4 Zr2 Zr1 90.3(3) . 2_565
O4 Zr2 Zr1 35.2(2) 20_565 2_565
O1 Zr2 Zr1 110.1(2) . 2_565
O1 Zr2 Zr1 164.8(3) 14 2_565
O1 Zr2 Zr1 74.4(3) 20_565 2_565
O1 Zr2 Zr1 110.6(3) 11_565 2_565
O3 Zr2 Zr1 35.2(2) . 2_565
O3 Zr2 Zr1 89.9(3) 14 2_565
Zr1 Zr2 Zr1 90.44(8) 14 2_565
Zr1 Zr2 Zr1 60.15(7) 13_565 2_565
O4 Zr2 Zr1 35.2(2) . .
O4 Zr2 Zr1 90.3(3) 20_565 .
O1 Zr2 Zr1 74.4(3) . .
O1 Zr2 Zr1 110.6(3) 14 .
O1 Zr2 Zr1 110.1(2) 20_565 .
O1 Zr2 Zr1 164.8(3) 11_565 .
O3 Zr2 Zr1 35.2(2) . .
O3 Zr2 Zr1 89.9(3) 14 .
Zr1 Zr2 Zr1 60.15(7) 14 .
Zr1 Zr2 Zr1 90.44(8) 13_565 .
Zr1 Zr2 Zr1 60.36(8) 2_565 .
O7 Mo3 O7 154(4) . 14
O7 Mo3 S5 100.3(15) . .
O7 Mo3 S5 100.3(15) 14 .
O7 Mo3 S5 100.3(15) . 8
O7 Mo3 S5 100.3(15) 14 8
S5 Mo3 S5 74(10) . 8
O7 Mo3 Zr1 43.4(14) . .
O7 Mo3 Zr1 111(2) 14 .
S5 Mo3 Zr1 132(4) . .
S5 Mo3 Zr1 132(4) 8 .
O7 Mo3 Zr1 111(2) . 14
O7 Mo3 Zr1 43.4(14) 14 14
S5 Mo3 Zr1 132(4) . 14
S5 Mo3 Zr1 132(4) 8 14
Zr1 Mo3 Zr1 67.4(12) . 14
Mo3 O7 Zr1 97(7) . .
O6 Mo2 O6 111(4) 2_565 .
O6 Mo2 Mo2 56.9(19) 2_565 2_565
O6 Mo2 Mo2 56.9(19) . 2_565
O6 Mo2 O3 86(2) 2_565 2_565
O6 Mo2 O3 86(2) . 2_565
Mo2 Mo2 O3 98.5(14) 2_565 2_565
O6 Mo2 S3 87(3) 2_565 .
O6 Mo2 S3 87(3) . .
Mo2 Mo2 S3 68.9(18) 2_565 .
O3 Mo2 S3 167(3) 2_565 .
O6 Mo2 S4 123(2) 2_565 .
O6 Mo2 S4 123(2) . .
Mo2 Mo2 S4 148(5) 2_565 .
O3 Mo2 S4 113(5) 2_565 .
S3 Mo2 S4 79(5) . .
O6 Mo2 Zr1 42.8(16) 2_565 2_565
O6 Mo2 Zr1 102(3) . 2_565
Mo2 Mo2 Zr1 74.4(10) 2_565 2_565
O3 Mo2 Zr1 43.5(8) 2_565 2_565
S3 Mo2 Zr1 128.7(18) . 2_565
S4 Mo2 Zr1 130(3) . 2_565
O6 Mo2 Zr1 102(3) 2_565 .
O6 Mo2 Zr1 42.8(16) . .
Mo2 Mo2 Zr1 74.4(10) 2_565 .
O3 Mo2 Zr1 43.5(8) 2_565 .
S3 Mo2 Zr1 128.7(18) . .
S4 Mo2 Zr1 130(3) . .
Zr1 Mo2 Zr1 69.9(12) 2_565 .
Mo2 S3 Mo2 42(4) 2_565 .
O5 Mo1 S1 70(2) . .
O5 Mo1 S1 70(2) 14 .
O4 Mo1 S1 154(3) 8 .
O5 Mo1 S2 127(2) . .
O5 Mo1 S2 127(2) 14 .
O4 Mo1 S2 117(3) 8 .
S1 Mo1 S2 89(3) . .
O4 Mo1 Mo1 90.8(14) 8 8
O5 Mo1 Zr1 47.0(13) . .
O5 Mo1 Zr1 99(2) 14 .
O4 Mo1 Zr1 46.3(9) 8 .
S1 Mo1 Zr1 115.8(18) . .
S2 Mo1 Zr1 133(2) . .
Mo1 Mo1 Zr1 66.1(9) 8 .
O4 Mo1 Zr1 46.3(9) 8 14
Zr1 Mo1 Zr1 72.6(13) . 14
S5 S5 Mo3 53(6) 8 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 O1 1.240(18) .
C1 O2 1.312(17) .
C1 C2 1.47(2) .
C2 C7 1.373(19) .
C2 C3 1.42(2) .
C3 C4 1.39(2) .
C4 C5 1.37(2) .
C5 C6 1.38(2) .
C5 C9 1.48(2) .
C6 C7 1.39(2) .
C8 C9 1.311(18) .
C8 C9 1.312(18) 19
C9 C10 1.38(2) .
C10 C11 1.419(19) .
C10 C12 1.53(2) .
C11 C11 1.55(4) 14_556
C12 C12 1.44(3) 14_556
O1 Zr2 2.187(10) .
O2 Zr1 2.208(9) .
O3 Zr1 2.130(9) 2_565
O3 Zr1 2.130(9) .
O3 Zr2 2.230(15) .
O3 Mo2 2.37(6) 2_565
O4 Zr1 2.154(9) 14
O4 Zr1 2.154(9) .
O4 Zr2 2.159(15) .
O4 Mo1 2.08(6) 8
O5 Mo1 1.72(4) 8
O5 Mo1 1.72(4) .
O5 Zr1 2.201(15) .
O6 Mo2 1.52(3) 2_565
O6 Mo2 1.52(3) .
O6 Zr1 2.227(15) .
Zr1 O7 2.201(10) .
Zr1 Mo1 2.98(4) 8
Zr1 Mo1 2.98(4) .
Zr1 Mo2 3.09(5) 2_565
Mo3 O7 2.0(2) .
Mo3 O7 2.0(2) 14
Mo3 S5 1.9(2) .
Mo3 S5 1.9(2) 8
Mo2 Mo2 1.67(11) 2_565
Mo2 S3 2.31(11) .
Mo2 S4 2.52(13) .
S1 Mo1 2.65(10) .
S1 Mo1 2.65(10) 8
Mo1 S2 2.73(11) .
Mo1 Mo1 2.42(10) 8
S5 S5 2.3(4) 8
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O1 C1 C2 C7 1(2) . .
O2 C1 C2 C7 -176.4(14) . .
O1 C1 C2 C3 -177.1(14) . .
O2 C1 C2 C3 6(2) . .
C7 C2 C3 C4 2(2) . .
C1 C2 C3 C4 179.9(15) . .
C2 C3 C4 C5 -2(3) . .
C3 C4 C5 C6 1(3) . .
C3 C4 C5 C9 -176.3(16) . .
C4 C5 C6 C7 0(3) . .
C9 C5 C6 C7 177.7(15) . .
C3 C2 C7 C6 -1(2) . .
C1 C2 C7 C6 -178.8(15) . .
C5 C6 C7 C2 0(3) . .
C9 C8 C9 C10 1(4) 19 .
C9 C8 C9 C5 -179.9(17) 19 .
C4 C5 C9 C8 124(2) . .
C6 C5 C9 C8 -54(3) . .
C4 C5 C9 C10 -57(3) . .
C6 C5 C9 C10 125.6(19) . .
C8 C9 C10 C11 -2(3) . .
C5 C9 C10 C11 178.7(19) . .
C8 C9 C10 C12 173(2) . .
C5 C9 C10 C12 -6(3) . .
C9 C10 C11 C10 3(4) . 19
C12 C10 C11 C10 -172.3(14) . 19
C9 C10 C11 C11 -179.8(13) . 14_556
C12 C10 C11 C11 5(2) . 14_556
C9 C10 C12 C12 180.0(15) . 14_556
C11 C10 C12 C12 -5(2) . 14_556
O2 C1 O1 Zr2 3(2) . .
C2 C1 O1 Zr2 -173.4(9) . .
O1 C1 O2 Zr1 -4(2) . .
C2 C1 O2 Zr1 172.5(9) . .
Mo2 O6 Mo2 O6 18(5) 2_565 2_565
Zr1 O6 Mo2 O6 -85(3) . 2_565
Zr1 O6 Mo2 Mo2 -103.4(18) . 2_565
Mo2 O6 Mo2 O3 102.7(17) 2_565 2_565
Zr1 O6 Mo2 O3 -0.7(18) . 2_565
Mo2 O6 Mo2 S3 -67(2) 2_565 .
Zr1 O6 Mo2 S3 -170.3(10) . .
Mo2 O6 Mo2 S4 -142(5) 2_565 .
Zr1 O6 Mo2 S4 115(6) . .
Mo2 O6 Mo2 Zr1 62(3) 2_565 2_565
Zr1 O6 Mo2 Zr1 -41(2) . 2_565
Mo2 O6 Mo2 Zr1 103.4(18) 2_565 .
Mo1 O5 Mo1 O5 4(4) 8 14
Zr1 O5 Mo1 O5 102.1(19) . 14
Mo1 O5 Mo1 O4 -89(2) 8 8
Zr1 O5 Mo1 O4 9.6(14) . 8
Mo1 O5 Mo1 S1 72(2) 8 .
Zr1 O5 Mo1 S1 169.9(10) . .
Mo1 O5 Mo1 S2 144(3) 8 .
Zr1 O5 Mo1 S2 -118(4) . .
Zr1 O5 Mo1 Mo1 98(2) . 8
Mo1 O5 Mo1 Zr1 -98(2) 8 .
Mo1 O5 Mo1 Zr1 -43(3) 8 14
Zr1 O5 Mo1 Zr1 55.7(13) . 14
